SET UP CONTROL OF SUPERPLASTIC FORMING OF ALUMINUM
ALLOYS AND STRATEGY FOR RHEOLOGICAL CHARACTERIZATION
OF MATERIALS BY BULGE TEST
Erick Petta Marinho, email@example.com
Fbio Cruz Ribeiro, firstname.lastname@example.org
Gilmar F. Batalha, email@example.com Laboratory of Manufacturing Engineering - Dept. of Mechatronics and Mechanical Systems Engineering - Escola Politcnica -
Universidade de So Paulo - Av. Prof. Mello Moraes, 2231- CEP 05508970 - So Paulo - Brazil
Abstract The aim is to propose the set up control of superplastic forming of aluminum alloys in an autoclave and a new strategy
for rheological characterization of materials by bulge test. The approach consists of a brief review of the basic
theoretical concepts of Superplastic forming. The methodology is divided into three control systems: (a) thermal cycle,
(b) pressurization cycle and (c) variation of strain rate. The development of the controls listed includes the activities
related to the design of the sensors, the setting of the plant control system, definition of the system data acquisition up
to the monitoring of process variables in real time, such as: temperature, pressure and deformation. New rheological
strategy here means choosing forming conditions, determining the pressure cycle, description of the rheological test
methods to determine the coefficients of interest (m, n and K). Based on the superplastic forming theory, it can be
concluded that it is very difficult to control all the variables used to explain this process. For Superplastic forming,
many steps of mechanical forming are reduced, with their corresponding time and cost savings. The process is widely
applied in aluminum alloys. The value of this paper is to summarize the main features, to explain the modeling chosen
and to propose a new strategy for rheological characterization of materials by bulge test.
Keywords: Superplasticity, Superplastic forming, instrumentation. Rheological characterization. Control.
In the economic and environmental global situation, growing fossil fuel price, lack of flexibility in alternative fossil
fuels, pollution and global warming represent a growing pressure in many industrial sectors, and the automobile sector
efforts focus on reducing fuel consumption and emission rates; so as to attain this goal, it is necessary to reduce the car
mass, and this requires a more extensive use of lightweight metal alloys. The barrier of the automobile industry is also
felt in the aeronautic industry. In this context, the successful use of titanium and aluminum alloys in aerospace projects
pushes some new technology processes forward, such as Superplastic forming.
Many studies on the phenomenon of superplasticity have been conducted, considering the period technological
limitations of the research, and they were important for establishing the limits to the use of this forming process.
Since the pioneer work by Bengough in 1912 (Bengough, 1912), the Superplastic phenomenon has been observed;
however, the first results obtained are attributed to Pearsons work (Fig. 1) in 1934 (Pearson, 1934), with superplastic
deformation of 1950% elongation in Bi-Sn alloy (it is worth noting that this material presents 5% elongation before
rupture outside superplastic conditions, being classified as fragile).
Fig. 1 - Pearson 1934, Bi-Sn alloy (1950%) (Pearson, 1934)
ABCM Symposium Series in Mechatronics - Vol. 5 Copyright 2012 by ABCM
Section II Control Systems Page 380
Bochvar (Bochvar & Sviderskaya, 1946), to whom the term superplasticity was attributed, based on the studies of
Pearson (Pearson, 1934), made their research in the 1940s. Researches were resumed in the West, only in 1962, after
the publication by Underwood (Underwood, 1962) for a Soviet review.
Before 1964, the research focus was on finding the maximum stretching through hot uniaxial tensile tests. The
focus on technological research began only after the pioneering work by Backofen (Backofen, Turner, & Avery, 1964);
the exponent m (strain rate sensitivity coefficient) began to be examined in more depth. Backofen, Turner & Avery, in
1964, from the MIT, published their much known paper in which, for the first time, a sheet of Superplastic AlZn
eutectoid alloy was pneumatically formed as a bubble. This event marks the emergence of a new technology:
Prof. Backofen and his research group at the Massachusetts Institute of Technology made a replication of the
Russian work and established the strain rate sensitivity importance as the neck-free tensile elongation characteristic of
superplastic metals. They also investigated other alloy systems, such as titanium, copper and magnesium.
Davis Stuart Fields was granted his PhD in metallurgy by MIT in 1957, and co-authored several papers with
When Backofen published in 1964, Dr. Fields was working at IBM Office Products Division in Lexington,
Kentucky, and he discovered the extraordinary formability possible with superplastic metals through Backofens work
at an ASM meeting.
By April 1965, Fields had written the worlds first superplastic forming patent application using a large range of
sheet- and tube-forming techniques formerly used for thermoforming plastics. After that, Fields (Fields & Stewart,
1971) studied the uniaxial tension ZnAl eutectoid alloy and the results were related to the thickness distribution in
All this work being developed in the USA was soon to be noted by the world scientific community.
The Electricity Council Research Center, Capenhurst, was the first industry with laboratories to study SPF. In 1969,
the first conference on SPF was held in Capenhurst. The participation of some groups, including some from Hinxton
Hall, Cambridge, British Aluminium Research Division and Press Steel Fisher Division of British Leyland, was
In 1971, ISC Alloys Ltd., Avonmouth Bristol, UK, was founded as the first commercial superplastic forming
company in the world; the motivation was the production of complex-shaped components using ZnAl eutectoid alloy
with low-cost tooling and forming times.
Immediately after the first demonstration of superplasticity in a dilure-aluminum alloy, in 1969, much development
activity was undertaken to scale up the special processing requirements needed to achieve a viable production route.
So far, the largest uniform elongation in uniaxial tension has been approximately 8000% achieved with commercial
bronze. This is clearly depicted in Fig. 2.
Fig. 2 - 1970, the turning point (Vulcan, 2006)
In the early 1970s, another development was also underway within the Aerospace Industry; this was the SPF of
titanium alloy and the new concept now known as SPF/DB, two-process combined SPF and diffusion bonding (DB).
This technology advanced considerably throughout the 1970s and early 1980s with the aid of government funding.
The first truly commercial application of SPF titanium was in 1981, some 13 years after Johnson had first
demonstrated SPF with a titanium alloy. This first commercial application was a jack housing produced by British
Aerospace Filton for the A310 Airbus aircraft. (Barnes, 2007)
ABCM Symposium Series in Mechatronics - Vol. 5 Copyright 2012 by ABCM
Section II Control Systems Page 381
Fig. 3 - Aluminum alloy EN AW 7475 superplastic forming (Robert, 2009)
Aluminium alloys (Fig. 3) used for superplastic forming are mostly known by their brand name or the name of the
product in the market. In automotive construction, aluminium alloy AA5083 is used for the internal parts of automotive
industry with superplastic forming. There are many companies in the market today that provide this material with
different names; Table 1 lists some of them:
Table 1 - List of companies and trade names for the aluminium alloy AA5083. (Vulcan, 2006)
Company Commercial names
Sky Aluminium ALNOVI-1
Fig. 4 illustrates the application of aluminum alloy in several industrial areas. (Vulcan, 2006)
Fig. 4 - Market distribution for aluminum alloy superplasticity forming pieces. (Vulcan, 2006)
The SPF titanium production expanded in the 1980s. Just 10 years later, in 1991, one aerospace contractor, Rohr
Industries, Chula Vista, had 10 full-time production presses and was producing more than 400 different part numbers at
an annual output of more than 20,000 SPF titanium parts. (Barnes, 2007)
Due to the rapid progress in this area in recent years, research into a larger number of materials besides that into
metallic materials (Chokshi, Mukherjee, & Langdon, 1993) also increased, such as ceramics, composites, intermetallic,
and more recently nanomaterials (Xu, 2009).
Nowadays, there are many innovations associated with superplasticity. The goal is a fully controlled process; it
means that all the variables of the process, such as temperature, strain rate and position (in some cases, tool movement)
must be controlled to optimize this already known process.
3. SUPERPLASTIC FORMING
3.1 Technological and economic factors
The hardening of material is practically inexistent and spring-back is zero; these features characterise a very good
finished product, with dimension